## the Nonlinear Response of Periodic Truss Lattices

Thesis by

### Gregory P. Phlipot

In Partial Fulfillment of the Requirements for the

Degree of

Doctor of Philosophy

CALIFORNIA INSTITUTE OF TECHNOLOGY

Pasadena, California

2019

c

2019

Gregory P. Phlipot ORCID: 0000-0003-2721-8678

### ACKNOWLEDGEMENTS

First and foremost, I would like to thank my advisor, Dr. Dennis Kochmann.

After attending his computational mechanics course my first year at Caltech

and seeing the high-quality research in his group, I knew that I wanted to work with him for my PhD. I was lucky enough to receive his excellent mentorship

and guidance over the next four years, which consisted of many fruitful and

though-provoking discussions. Even after accepting his current position at

ETH and moving to Zürich, Dennis always made time in his busy schedule

to be available to talk and guide me in the right direction, which I deeply

appreciate. I would also like to thank my committee members, Dr. Michael

Ortiz, Dr. Chiara Daraio, and Dr. Domniki Asimaki, for their time and effort

spent participating in my defense, as well as their well-informed feedback.

I would like to express my gratitude to all of the professors who challenged

me with meaningful research or coursework during my time at Arizona State

and at Caltech. Specifically, I would like to thank Dr. Marc Mignolet, who

convinced me to work on research during my undergraduate degree, persuaded

me to pursue a PhD, and got me interested in research and the field of

com-putational mechanics.

I would also like to thank all of the members of the Kochmann Research Group

— both past and present — for all of the excellent discussions during group meetings and around the office. Alex Zelhofer and Ishan Tembhekar were

especially welcoming when I joined the group and helped me with both research

and non-research related matters. I would also like to extend a special thank

you to the group members and friends at ETH, especially Abbas Tutcuoglu

and Raphaël Glaesener, for making me feel at home during my two-month

visit to Zürich. Danke.

There is no doubt in my mind that I would not have been able to complete my degree if it wasn’t for all of my colleagues and friends at Caltech. Whether

it was helping me finish up homework at midnight while sitting in our shared

first-year office, keeping me company everyday at lunch, or letting go on one

of our quasi-yearly trips to Las Vegas, they supported me along the way and

helped me maintain the right amount of work-life balance needed to complete

Lastly, I would like to thank my parents, Sue and Mike Phlipot, for instill-ing the importance of education, inspirinstill-ing me to become an engineer, and

supporting me throughout my schooling.

### ABSTRACT

We present a framework for the efficient, yet accurate description of general

pe-riodic truss networks based on concepts of the quasicontinuum (QC) method.

Previous research in coarse-grained truss models has focused either on simple bar trusses or on two-dimensional beam lattices undergoing small

deforma-tions. Here, we extend the truss QC methodology to nonlinear deformations,

general periodic beam lattices, and three dimensions. We introduce geometric

nonlinearity into the model by using a corotational beam description at the

level of individual truss members. Coarse-graining is achieved by the

intro-duction of representative unit cells and a polynomial interpolation analogous

to traditional QC. General periodic lattices defined by the periodic assembly

of a single unit cell are modeled by retaining all unique degrees of freedom of

the unit cell (identified by a lattice decomposition into simple Bravais lattices) at each macroscopic point in the simulation, and interpolating each degree

of freedom individually. We show that this interpolation scheme accurately

captures the homogenized properties of periodic truss lattices for uniform

de-formations. In order to showcase the efficiency and accuracy of the method,

we compare coarse-grained simulations to fully-resolved simulations for

vari-ous test problems, including: brittle fracture toughness prediction, static and

dynamic indentation with geometric and material nonlinearities, and uniaxial

tension of a truss lattice plate with a cylindrical hole. We also discover the

notion of stretch locking — a phenomenon where certain lattice topologies are

over-constrained, resulting in artificially stiff behavior similar to volumetric locking in finite elements — and show that using higher-order interpolation

instead of affine interpolation significantly reduces the error in the presence

of stretch locking in 2D and 3D. Overall, the new technique shows convincing

agreement with exact, discrete results for a wide variety of lattice

architec-tures, and offers opportunities to reduce computational expenses in structural

lattice simulations and thus to efficiently extract the effective mechanical

### PUBLISHED CONTENT AND CONTRIBUTIONS

[1] Gregory P. Phlipot and Dennis M. Kochmann. A quasicontinuum theory for the nonlinear mechanical response of general periodic truss lattices.

### TABLE OF CONTENTS

Acknowledgements . . . iii

Abstract . . . v

Published Content and Contributions . . . vi

Bibliography . . . vi

Table of Contents . . . vii

List of Illustrations . . . ix

List of Tables . . . xvii

Chapter I: Introduction . . . 1

1.1 Overview of Microstructured Materials . . . 1

1.2 Outline of this Thesis . . . 4

1.3 Finite-Sized Truss Structures . . . 5

1.4 Brief Overview of Homogenization Theory . . . 7

1.5 Properties of Periodic Truss Lattices . . . 10

Chapter II: Numerical Modeling of Truss Structures . . . 16

2.1 High-Fidelity RVE Characterization . . . 16

2.2 Fully-Resolved Simulations . . . 17

2.3 Numerical Homogenization . . . 18

2.4 Quasicontinuum Method . . . 20

2.5 Shortcoming of Existing Methods . . . 23

Chapter III: Fundemantals of the Quasicontinuum Method . . . 26

3.1 Initial Problem Statement . . . 26

3.2 Modeling Individual Truss Members . . . 29

3.3 History-Dependent Problems . . . 36

3.4 The Quasicontinuum Method . . . 43

3.5 Adaptive Refinement . . . 51

3.6 Comparison with FE2 _{and classical homogenization} _{. . . .} _{52}

Chapter IV: Applications . . . 54

4.1 Elastic Constants . . . 54

4.2 Boundary Layer Method . . . 60

4.3 Indentation . . . 66

4.4 Dynamic Indentation . . . 70

4.5 Hole in Plate Made of an Elasto-Plastic Truss Lattice . . . 75

Chapter V: Higher-Order Quasicontinuum Techniques and Stretch Locking 80 5.1 Stretch Locking . . . 80

5.2 Higher-Order Interpolation and Summation Rules . . . 82

5.3 Performance of Higher-Order Methods . . . 89

Chapter VI: Numerical Considerations . . . 101

6.1 Structure of a Simulation . . . 101

Chapter VII: Discussion and Outlook . . . 117

7.1 Accomplishments . . . 117

7.2 Future Work . . . 119

Bibliography . . . 123

Appendix A: Effective Elastic Constants of Periodic Truss Lattices . . 137

### LIST OF ILLUSTRATIONS

Number Page

1.1 Scanning electron micrographs of natural materials with a

me-chanical microstructure, taken from [48] . . . 1

1.2 Examples of periodic truss lattices: Ultralight hollow metallic

microlattice [93] (left), solid carbon lattice reprinted by

permis-sion from Springer Nature: Nature Materials [12], copyright 2016

(center), and a hierarchical lattice reproduced from [70](right). 3

1.3 Examples of rigid and non-rigid truss structures. On the left, a rigid truss structure satisfying the necessary conditions for static

and kinematic determinacy with no states of self-stress or

mech-anisms. In the center is a truss structure that does not satisfy

Maxwell’s inequality, and thus has a mechanism (shown in dotted

lines). On the right, a truss structure that satisfies the necessary

conditions for static and kinematic determinacy, but has both a

mechanism and a state of self-stress. . . 7

1.4 Two-scale nonlinear elasticity boundary value problem with

es-sential boundary conditions and applied tractions T. As the characteristic size of the unit cell ε tends towards zero,

homoge-nization attempts to find a smooth homogenized energy density

W(∇u) to approximate the highly oscillatory energy density of the . . . 8

1.5 The unit cell problem with periodic boundary conditions. The

average deformation gradient of the macroscale F is applied to

the unit cell, and the fine-scale correction v is determined by

minimizing the energy of the unit cell over all periodic corrections. 9

1.6 Categorizing lattices and bending- or stretching-dominated lat-tices and as Bravais latlat-tices or multilatlat-tices. . . 12

1.7 Depiction of the boundary layer method for a cellular material.

Reprinted by permission from Springer Nature: International

1.8 Elastic moduli and yield strength of various materials. Note that the predicted stiffness and strength of lattices made of aluminum

or carbon fiber reinforced polymers (CRFP) populate otherwise

empty regions of the material space. Reproduced from Fleck

et al. [40] with permission of the copyright holder, The Royal

Society. . . 15

2.1 Computed homogenized stiffness of solid (left) and hollow shell

(right) octet truss lattices using continuum-level finite element

analysis (with the commercial code Abaqus), and structural

Euler-Bernoulli and Timoshenko beams for various relative densities. Reprinted from [71]. . . 17

2.2 Simulation of uniaxial tension of a notched hollow octet truss

lattice modeled using shell finite elements to investigate the

in-sensitivity of truss lattices to flaws. Reprinted from [73]. . . 18

2.3 Pictorial description of numerical homogenization reprinted from

Matouš et al. [67] with permission of the copyright holder,

Else-vier. FM represents the macroscopic deformation gradient, and

SM and CM represent the macroscopic stress and tangent

ma-trices that are returned to the macroscale after solving the RVE

problem. . . 19 2.4 The traditional QC method for atomic lattices (left) and the

extension to truss lattices (right). . . 21

2.5 The QC method paired with aspects of the extended finite

ele-ment method to model the crack propagation (crack path shown

in red) in a cross-braced truss lattice. Reprinted from Rokoš

et al. [88] with permission from the copyright holder, Elsevier . 24

3.1 (a) Example definition of a unit cell Ωu based on its node(s)

(solid circle) and its connecting beams En

u (in this case Eu =

∅). Further shown are examples of (b) a simple Bravais lattice (diamond) and (c) a multilattice (hexagon, composed of two simple Bravais lattices) and their corresponding unit cells and

unit cell dofs. The dofs of all nodes inside each unit cell are

3.2 Kinematics of the 3D corotational beam: the linear Euler Bernoulli beam rotates with the element frame Rb, and has small angle

deflections at each node. Superscripts r, u, d, and b stand for

the (r)eference, (u)ndeformed, (d)eformed, and (b)eam

configu-ration, respectively. . . 33

3.3 Example stress-strain curve for the plasticity model with isotropic

hardening. Reprinted by permission from Springer Nature: Springer

Computational Inelasticity by J.C. Simo and T.J.R. Hughes,

copyright 2000 [97]. . . 39

3.4 Illustration of the interpolated dofs and the recovery of nodal dofs within individual unit cells from the interpolation: (a)

shows a mesh of coarse-grained/macroscopic elements whose

ver-tices are repUCs that carry dofs ϕ. (b) Within an element K, the dofs ϕare interpolated by evaluating the shape functions at

each unit cell location, e.g. Xi or Xj (in the reference

configu-ration). (c)Dofs {ϕ0,ϕ1}of the two nodes within each unit cell are recovered from the interpolated repUC dofs. . . 44

3.5 First and second-order summation rules. The first-order

sum-mation rule (left) shows the vertex sampling unit cells (blue)

and the local inner sampling unit cell (red). The second-order summation rule (right) also has edge sampling unit cells (green). 48

4.1 Unit cells of lattices with (a) square, (b) hexagon, (c) kagome,

(d) triangle, (e) star-shaped 2D, (f) cubic, (g) cuboctahedron,

and (h) BCC architecture. . . 55

4.2 Representative, randomly coarse-grained truss QC simulations in

2D and 3D for the elastic constant calculation: (left) a coarse-grained hexagon lattice with 30% repUC density and (right) a bcc lattice with 10% repUC density. Affine boundary conditions are applied to the translational dofs on the outer faces of the block, and the energy of all sample unit cells inside the yellow

box is used to calculate the elastic modulus (the large region in

4.3 Errors in the linear elastic bulk, shear, and uniaxial moduli of 2D lattices at 20% (solid markers) and 1% (hollow markers)

rel-ative density, computed by coarse-grained truss QC simulations

with the first-order (left) and second-order (right) optimal sum-mation rule and random repUC selection for each level of repUC

density. Markers correspond to the average error from 20 ran-domly coarsened meshes, and the bars represent the standard

deviations of the errors. . . 58

4.4 Errors in the linear elastic bulk, shear, and uniaxial moduli of

3D lattices at 20% (solid markers) and 1% (hollow markers) rel-ative density, computed by coarse-grained truss QC simulations

with the first-order (left) and second-order (right) optimal sum-mation rule and random repUC selection for each level of repUC

density. Markers correspond to the average error from 20 ran-domly coarsened meshes, and the bars represent the standard

deviations of the errors. . . 59

4.5 Coarse-grained kagome lattice in 2D with a pre-existing crack

undergoing mode-I loading, simulated by truss QC with

adap-tive mesh refinement. The colors correspond to the (normalized)

maximum tensile stresses in the beams. . . 62 4.6 Fully-resolved simulation of the 2D kagome lattice undergoing

mode 1 loading. The colors correspond to the (normalized)

max-imum tensile stresses in the beams. . . 63

4.7 Convergence of the maximum strut tensile stress near the notch

tip (left) and of the total energy (right) as compared to the fully-resolved simulation for coarse-grained truss QC fracture

simula-tions of a (top) kagome lattice, (bottom) triangle lattice in 2D. Insets visualize the adaptively refined QC representation at the

indicated repUC densities. . . 64 4.8 Convergence of the maximum strut tensile stress near the notch

tip (left) and of the total energy (right) as compared to the fully-resolved simulation for coarse-grained truss QC fracture

simula-tions of a (top) hexagon lattice, (bottom) star-shaped lattice in 2D. Insets visualize the adaptively refined QC representation at

4.9 Initial geometry for the fully-resolved (left) and coarse-grained (right) 2D kagome lattice before indentation. . . 67 4.10 (a)Normalized load-displacement curves for the indentation into

a 2D kagome lattice, (b) the repUC density as the simulation progresses, and the final deformed configurations of the(c) fully-resolved Euler-Bernoulli beam, (d) fully-resolved corotational beam, and(e)adaptively refined corotational beam simulations. The colors of beams correspond to the maximum tensile stress

in each beam normalized by Young’s modulus. . . 69

4.11 (a)Initial geometry for the fully-resolved and(b)coarse-grained truss QC of a 3D kagome lattice before indentation. . . 70

4.12 Normalized load-displacement curve for the indentation of a 3D

kagome lattice (top left), the repUC density as the simulation progresses (top right), and the slices of the final deformed config-urations of the fully-resolved (bottom left) and adaptively refined (bottom right) simulations with average axial strain contours. . 71 4.13 Geometry of the coarse-grained dynamic indentation simulation.

The left shows the initial coarse-grained truss lattice with the

mesh and sample unit cells. . . 72

4.14 Snapshots of the truss lattice: coarse-grained (left) and fully-resolved (right). Colors correspond to the maximum stress in

each beam, and the broken beams are not shown. . . 74

4.15 Magnitude of the acceleration in the coarse-grained (left) and

fully-resolved (right) simulations at various time steps before

fail-ure of the truss lattice. The elastic waves can be seen artificially

bounding off mesh boundaries in the coarse-grained simulations. 76

4.16 Cylindrical hole in octet lattice plate. The fully-resolved truss

lattice (left) and the coarse-grained mesh (right) . . . 77

4.17 Average stress-strain relation for the octet truss hole-in-plate ex-tension simulations with first- and second-order summation rules,

compared with the fully-resolved simulation. The insets are

col-ored by the axial stress in each bar in the specimen at

4.18 Plastic strains near the cylindrical hole at 20% macroscopic strain for the coarse-grained simulations with first-order summation

rule (top), second-order summation rule (middle), and the fully-resolved simulation (bottom). The maximum plastic strains are 0.597 (coarse-grained, first-order summation) 0.632 (coarse-grained,

second-order summation), and 0.627 (fully-resolved). . . 79

5.1 Traditional Cook’s membrane geometry (left) and the corre-sponding hexagon lattice membrane (right) with each truss mem-ber having a length of L= 1. . . 81 5.2 Example meshes for the coarse-grained truss lattice Cook’s

mem-brane simulations. Full resolution (top), coarsening of n = 4

(bottom left), and coarsening of n = 8 (bottom right) of the 2D kagome lattice. . . 83

5.3 Normalized strain energy of truss lattice versions of Cook’s

mem-brane problem for various 2D truss topologies with relative

den-sity ρ¯= 1%. Insets show the deformed fully-resolved and coarse-grained (with repUC density of1/9) simulations of the hexagon(top) and star-shaped (bottom) lattices, colored by the displacements normalized by the maximum displacement of the fully-resolved

truss. . . 84 5.4 Strain energy of the hexagon and star-shaped lattices at relative

densities of ρ¯= 10% and ρ¯= 1%. . . 85 5.5 An example of higher-order interpolation QC used to model

bending of planar lattices (left, reprinted from [16] with per-mission of the copyright holder, Elsevier), and an example of a

quadratic tetrahedron in the QC method used to model a "lattice

continuum" (right). . . 85 5.6 Example of the proposed higher-order interpolation strategy

ap-plied to a square lattice. The underlying truss lattice (grey) is approximated using the repUCs (blue) connected by the mesh

5.7 Errors in the linear elastic bulk, shear, and uniaxial moduli of 2D lattices at 20% (solid markers) and 1% (hollow markers)

rel-ative density, computed by coarse-grained truss QC simulations

with quadratic interpolation paired with quadrature (left) and optimal (right) summation rules and random repUC selection for each level of repUC density. Markers correspond to the average

error from20randomly coarsened meshes, and the bars represent the standard deviations of the errors. . . 90

5.8 Errors in the linear elastic bulk, shear, and uniaxial moduli of

3D lattices at 20% (solid markers) and 1% (hollow markers) rel-ative density, computed by coarse-grained truss QC simulations

with quadratic interpolation paired with quadrature (left) and optimal (right) summation rules and random repUC selection for each level of repUC density. Markers correspond to the average

error from20randomly coarsened meshes, and the bars represent the standard deviations of the errors. . . 91

5.9 Normalized strain energy of the Cook’s membrane simulations of

the hexagon (top) and star-shaped (bottom) lattices with relative density of ρ¯ = 1%. The insets show the deformed membranes and are colored by the magnitude of displacements (normalized by the maximum displacement of the fully-resolved simulation). 93

5.10 Convergence of the strain energy and maximum tensile stress in a

strut near the notch tip for the hexagon and star-shaped lattice

coarse-grained boundary layer simulations using the quadratic

interpolation and the optimal (blue) and exact (orange)

summa-tion rules. . . 96

5.11 A lattice block with distributed shear load placed on the top.

The cube is made by tessellating either the tetrakaidecahedron(top right) or the 3D star-shaped (bottom right) unit cell. . . 97 5.12 Strain energy in the coarse-grained QC simulations of the

tetrakaidec-ahedron lattice block undergoing a distributed shear load across

the top surface. The insets show the deformed configurations of

all of the sampling unit cells, and are color-coded based on the

5.13 Strain energy in the coarse-grained QC simulations of the 3D star-shaped lattice block undergoing a distributed shear load

across the top surface. The insets show the deformed

config-urations of all of the sampling unit cells, and are color-coded

based on the displacements. . . 99

6.1 Program flow chart. . . 102

6.2 Examples of sampling truss elements (with small nodes) and

their corresponding energy sampling elements (with larger nodes).

The colors of the truss members match the nodes of the mesh

needed to compute the energy of the truss member (i.e. the re-pUCs with nonzero shape functions at the truss member nodes).

The number of nonzero shape functions can vary - examples of

truss members with 1 (green), 2 (yellow), 3 (red), and 4 (blue)

### LIST OF TABLES

Number Page

6.1 Time (in seconds) spent assembling and solving the lattice block

shear simulations in Section 5.3.4 with quadratic interpolation.

Simulations were performed on a machine with an Intel Xeon

CPU E5-2650 processor using 12 cores with 1 MPI process per core. . . 115

6.2 Time (in seconds) spent in different parts of the code for the

dynamic indentation simulations in Section 4.4. "Total Solve"

represents the total time in the nonlinear solver (i.e. assembling

systems, solving linear systems, and performing line searches).

Simulations were performed serially on a machine with an Intel

C h a p t e r 1

### INTRODUCTION

1.1 Overview of Microstructured Materials

Many materials that appear to be homogeneous — both natural and

en-gineered — have a mechanical microstructure that greatly influences their macroscopic properties. All materials have some sort of microstructure (e.g.

polymer networks, atomic grain structures), but by mechanical microstructure,

we mean structural features on a mesoscale larger than the typical

microstruc-tural scales, but on a much smaller scale than the macroscopic size of an

object. Two quintessential examples of naturally occurring materials with

me-chanical microstructure are wood and bone (see Fig. 1.1), but the properties

of other natural materials are also greatly influenced by their microstructure.

The microstructure in wood comes in the form of fibers, which give it its

char-acteristic anisotropy. On the other hand, bone has a seemingly random porous microstructure, which can lead to isotropic macroscopic properties.

Many engineered materials also make use of microstructure to obtain certain desirable macroscopic properties. The most common of these materials are

engineered foams. Foams can be made out of a variety of constituent materials,

but they are characterized by their cellular nature and random microstructure.

(a) Cancellous bone (b) Orthogonal slices of cedar wood along the axis of the fibers (left), and transverse to the fibers (right).

Foams are used in many products to achieve a wide variety of reasons, including

• Cars. Car bumpers utilize plastic foams to maximize energy dissipation in collisions.[95].

• Houses. Plastic foams are the most common thermal insulator used in buildings[25].

• Aerospace vehicles. The strong and lightweight nature of foams make them ideal core materials for sandwich panels commonly used in airplanes

[50].

• Mattresses. Memory foam (developed by NASA in the 1970s to im-prove seat cushioning) is commonly used to make comfortable beds [27].

An excellent overview of mechanical, acoustic, and electrical properties of

vari-ous microstructured materials (including foams, honeycombs, and natural

ma-terials) was presented in Gibson and Ashby [48].

Even though the manufacturing of foams and other materials with random

mi-crostructure has improved and enabled engineering feats like landing a rover

on Mars1, manufacturing materials with a designed, ordered microstructure has been out of reach until recently. The recent advances in additive manu-facturing techniques have enabled the creation of materials with an arranged

microstructure — commonly referred to as metamaterials2 _{— giving engineers}

the ability to design materials with virtually any microstructure.

One popular class of mechanical metamaterials are periodic truss lattices. In

part due to their manufacturability, and in part due to some of their desirable

theoretical properties, periodic truss lattices have garnered significant

inter-est in the past decade. Notably, a metal hollow microlattice manufactured

by HRL Laboratories in 2011 pushed the boundaries of ultralight materials by creating a metamaterial that is99.99%air [93]. There has also been pioneering work at smaller scales. Additive manufacturing techniques have been used to

1_{NASA’s Mars Science Laboratory spacecraft carried the Curiosity rover to the martian}
surface in 2012 using a Phenolic Impregnated Carbon Ablator (PICA) heat shield, which
inherits its desirable thermal properties in part from the microstructure of the material.

Figure 1.2: Examples of periodic truss lattices: Ultralight hollow metallic mi-crolattice [93] (left), solid carbon lattice reprinted by permission from Springer Nature: Nature Materials [12], copyright 2016 (center), and a hierarchical lat-tice reproduced from [70](right).

manufacture polymer lattices with sub-micrometer resolution [66]. Further-more, these polymer lattices have been coated with a thin layer of ceramic

and the polymer has been etched out, leaving an ultralight ceramic hollow

truss lattice with wall thicknesses as low as 5 nanometers [69]. In addition

to the standard periodic truss lattices, there has been interest in hierarchical

truss lattices [70, 115] (truss lattices made of truss lattices) as hierarchical

microstructures are seen in nature.

The ability to design and manufacture these multiscale materials leads directly

to two questions:

1. Given a certain microstructure and the properties of the constituent material, what are the effective properties at the macroscale?

2. Given desired macroscopic properties, what microstructure and

con-stituent material can be used to achieve the properties?

The first question is hereby referred to as theforward problem since it requires computing quantities given known inputs. Conversely, the second is referred

to as the inverse problem because it requires finding the inputs that give a desired output. Since solving the inverse problem requires solving the forward

problem, the decades-old field of extracting the effective macroscopic response

of microstructured materials has recently been revitalized by the advancements

in manufacturing. The theoretical foundation for the micromechanical

model-ing of metamaterials probably began with Hill [52] calculatmodel-ing of the effective,

of homogenization theory followed, including probabilistics and wave propa-gation [21] as well as nonlinearity [46].

While there has been significant work towards answering the forward problem,

the ability to predict the general nonlinear response of metamaterials (e.g.

buckling of truss members, densification, failure of microstructure components,

etc.) is still a challenge. This results in an expensive and slow design cycle

relying on excessive manufacturing and testing to span the design space looking

for microstructures that give desired properties. Ideally, this process could be

expedited using theoretical or computational models, such that solving the forward problem becomes inexpensive and fast. Then these models could be

used to span the design space of microstructures, and augment the design

process to solve the inverse problem. This is the motivation for the research

in this thesis.

1.2 Outline of this Thesis

The goal of this thesis is to develop a multiscale modeling technique that can

be used to efficiently and accurately model the nonlinear mechanical response

a particular type of metamaterial: periodic truss lattices. In the remainder

of this chapter, we give an overview of truss lattices including some previous

relevant theoretical results, and the experimental literature. Chapter 2

con-tains the fundamentals of numerical modeling of truss lattices and provides details on popular numerical methods and their shortcomings, motivating the

research in this thesis: an extension of the quasicontinuum (QC) method to

model complex trusses. Chapter 3 outlines the QC method and formulates the

extension of the method which represents the bulk of the research. Chapter 4

is composed of multiple test cases to show the usefulness of the previously

for-mulated QC method. One of the test cases shows a disagreement between the

QC method and fully-resolved simulations when it comes to predicting the

re-sponse of some bending-dominated lattices. This motivates Chapter 5, where

the notion ofstretch locking is investigated, and the previous QC formulation is modified by using higher-order interpolation functions in order to mitigate

this phenomenon, leading to a more accurate model. In Chapter 6, the

com-putational performance of the method is discussed, and the thesis concludes

1.3 Finite-Sized Truss Structures

Understanding the mechanical properties of trusses starts with understanding

the differences between the bending stiffness and axial stiffness of a beam. In

an undergraduate mechanics course, we learn that the tip displacements of a

cantilevered beam corresponding to a tip load F in the axial and transverse

directions are

∆x= F L

EA and ∆y=

F L3

3EI, (1.1)

respectively, where L is the length of the beam, E is the Young’s modulus

of the material, A is the cross-sectional area, and I is the moment of inertia. If the beam has a characteristic cross-section dimension r, the area of the

beam in three dimensions is proportional tor2_{, while the moment of inertia is}

proportional to r4_{. This means that the stretching and bending stiffness per}

unit length of a beam in 3D satisfy

k(3_{stretch}D) ∼r

L

2

and k_{bend}(3D)∼r

L

4

. (1.2)

Similar arguments for two-dimensional beams (where the out-of-plane

thick-ness of the beam is constant and independent of r) lead to

k_{stretch}(2D) ∼r

L

and k(2_{bend}D) ∼r

L

3

. (1.3)

Since trusses are assumed to be composed of slender beams (i.e. beams with

r/L 1), the axial, or stretching stiffness can be orders of magnitude larger than the bending stiffness.

For that reason, the concept of kinematically and statically determinate

struc-tures is important to understanding the mechanical properties of trusses. A

truss structure is said to bekinematically determinate if there are no kinemati-cally admissible deformations (excluding rigid body modes) such that no truss

member changes its length. Conversely, kinematically indeterminate trusses are defined as structures where there exists at least one kinematically

ad-missible deformation mode (excluding rigid body modes) such that no truss

members change length. Similarly, a structure is said to be statically deter-minate if there exist no (nonzero) stress states such that the net force on all nodes is zero, and astatically indeterminate structure has at least one nonzero stress state that results in zero forces on all nodes.

If the truss is statically indeterminate, the states of stress that produce a net

indeterminate, the deformation modes where no truss members change length are called mechanisms. They are called mechanisms since the truss is able to deform purely through bending of beams, which is orders of magnitude less

stiff than the stretching deformation modes. In fact, it is common to analyze

truss structures as pin-jointed bars, where the mechanisms are treated as

zero-energy modes. It is therefore common to refer to kinematically determinate

structures as rigid trusses, while kinematically indeterminate structures are

non-rigid.

A detailed formulation of statically and kinematically determinate truss

struc-tures is given in Pellegrino and Calladine [80], and is summarized here. Given

a truss structure with n nodes and b beams, a matrix A∈_{R}dn×b _{in}_{d} _{}

dimen-sions, called the equilibrium matrix, can be used to relate the displacements

of the nodes,u, to the elongations of the beams,e, according to

ATu =e. (1.4)

By using the principle of virtual work, the matrixAcan also be used to relate

the tensions in each bar, t, and the forces at each node, f, via

At=f. (1.5)

By the definitions of states of self-stress and mechanisms given above, the

states of self-stress satisfy the equation At=0, while the mechanisms satisfy

ATu = 0. In other words, the states of self-stress form the nullspace of A, while the mechanisms form the left nullspace ofA.

Therefore, the rigidity of a truss can be determined by the dimensionality of

the left nullspace of A. If dim(null(AT_{)) = 3} _{in 2D or} _{dim(null(}_{A}T_{)) = 6}

in 3D, then the only mechanisms are the rigid body modes, and the truss

structure is rigid. The dimension of the left nullspace of a matrix is at least as

large as the difference between the number of rows and columns in the matrix.

This leads directly to Maxwell’s relation for the necessary condition for a truss

lattice to be rigid [44],

b ≥2d−3 in 2D, and b≥3d−6 in 3D. (1.6)

Similar analysis with the states of self-stress lead to the necessary condition

for a truss to be statically determinate (i.e. there are no states of self-stress),

or

Figure 1.3: Examples of rigid and non-rigid truss structures. On the left, a rigid truss structure satisfying the necessary conditions for static and kinematic determinacy with no states of self-stress or mechanisms. In the center is a truss structure that does not satisfy Maxwell’s inequality, and thus has a mechanism (shown in dotted lines). On the right, a truss structure that satisfies the necessary conditions for static and kinematic determinacy, but has both a mechanism and a state of self-stress.

The combination of the two equations suggests that a necessary (but not

suffi-cient) condition for a truss to be both statically and kinematically determinate

is when the inequalities are satisfied as equalities. See Fig. 1.3 for examples of rigid and non-rigid truss structures. For more information on the

equilib-rium matrix, and how the four fundamental subspaces of Arelate to states of

self-stress and mechanisms, see Pellegrino and Calladine [80].

1.4 Brief Overview of Homogenization Theory

Due to the multiscale nature of periodic truss lattices, homogenization

tech-niques are used to understand the response of the effective material. One of the

most important homogenization problems for understanding the quasistatic

re-sponse of metamaterials is that of the two-scale nonlinear elasticity problem.

Since the conclusions drawn from the two-scale homogenization problem are

so important (and will be referenced throughout the thesis) we take the time here to outline the problem, go over key results, and show how the theory can

be applied to periodic truss lattices.

The macroscale boundary value problem of a heterogeneous bodyΩwith statis-tically homogeneous microstructure — represented by a representative volume

element (RVE) ΩUC — aims to identify the deformation mapping or

displace-ment field as the minimizer of the total potential energy

I[u] =

Z

Ω

Wx

,∇u

_{d}_{V} _{− L(}_{u}_{)} _{(1.8)}

con-Figure 1.4: Two-scale nonlinear elasticity boundary value problem with essen-tial boundary conditions and applied tractionsT. As the characteristic size of the unit cellε tends towards zero, homogenization attempts to find a smooth homogenized energy densityW(∇u)to approximate the highly oscillatory en-ergy density of the

ditions on ∂Ω2 (see Fig. 1.4). Here, W denotes the strain energy density as a

function of position x and the displacement gradient, L is the external force potential3, and is a characteristic size of the RVE. That is, we have

u= arg minI[u] | u ∈H_{0}1(Ω) , (1.9)

whereH1

0(Ω)⊂H1(Ω)is the set of functions satisfying the Dirichlet boundary

conditions.

Since the material’s constitutive response fluctuates on the scale of y = x/

whereas the boundary value problem (i.e. the geometry and any loading) varies

on the scale of x, one ideally seeks to find a homogeneous energy density

W∗(∇u) such that Eq. (1.8) converges to the homogeneous total potential energy

I[u] =

Z

Ω

W∗(∇u) dV − L(u), (1.10)

in some sense. In particular, it is desired that Eq. (1.8) Γ-converges to Eq. (1.10), which guarantees the convergence of minimizers of the functionals.

As shown in Geymonat et al. [46], if W(·,∇u) is convex, the homogenized energy density can be computed by solving the RVE problem

W∗(∇u) = inf

1 |ΩUC|

Z

ΩUC

W(y,∇u+∇v) dV | v ∈V(ΩUC)

, (1.11)

with V(ΩUC) ⊂ H1(ΩUC) being the set of all periodic H1-functions on ΩUC

with zero mean, i.e. R_{Ω}

UCvdV =0.

3_{In the case of Fig. 1.4, the external force potential is}_{L(u}_{) =}R

∂Ω2T·u

Figure 1.5: The unit cell problem with periodic boundary conditions. The average deformation gradient of the macroscale F is applied to the unit cell, and the fine-scale correction v is determined by minimizing the energy of the unit cell over all periodic corrections.

In the case of linear elasticity, the energy density is convex, and Eq. (1.11) holds

(see Cioranescu and Donato [30] for a detailed discussion of homogenization

in linear elasticity). However, for finite deformations, the energy density is in
general not convex4_{, and the homogenized energy density is given by}

W∗(∇u) = inf

k∈Z

inf

1 |kΩUC|

Z

kΩUC

W(y,∇u+∇v) dV | v ∈V(kΩUC)

,

(1.12)

where kΩUC is a kd sized tessellation of RVEs in d dimensions.

The single RVE problem in Eq. (1.11) is not difficult to solve, and can be

thought of as affinely deforming the RVE using the deformation gradient,

then allowing a periodic displacement field across the unit cell in order for

the RVE to "relax" (see Fig. 1.5). On the other hand, Eq. (1.12) requires

performing the same computation over an unbounded number of unit cells,

which is impractical, and is one of the reasons why homogenization of solids undergoing finite deformations is so difficult.

In order to use the aforementioned homogenization techniques for linear elastic

periodic truss lattices, the unit cell of the truss is used as the RVE. Then, the

truss members are either discretized with continuum finite elements or beam

finite elements, with the latter resulting in the discrete RVE problem

W(∇u) = inf u,θ

(

1 |ΩUC|

X

e∈E

We(u,θ)

)

s.t. u(X+)−u(X−) = ∇u(X+−X−)

θ(X+)−θ(X−) =0,

(1.13)

where We is the energy of an individual beam in the truss, u and θ are the

translational and rotational dofs of the beam finite elements, andX+ andX−

represent points on opposite sides of the unit cell. Since Eq. (1.13) usually has

relatively few degrees of freedom to minimize, the homogenized energy density

can sometimes be computed analytically. This was done for some 2D linear

elastic truss lattices, and the homogenized stiffness tensors in Voigt notation

are included in Appendix A.

1.5 Properties of Periodic Truss Lattices

1.5.1 Bending- and Stretching-Dominated Lattices

The analysis of kinematically determinate truss structures was extended to

the case of an infinite periodic truss lattice in Deshpande et al. [34]. Similar

counting of the number of beams and nodes used in Maxwell’s relation for an

infinite periodic truss leads to the necessary condition that the average number

of beams connected at each node must be Z = 4 in 2D or Z = 6 in 3D in order for a truss to be rigid. Note again that the connectivity of the truss is a

necessary, but not sufficient condition for rigidity.

Hutchinson and Fleck [54] looked at whether periodic truss lattices were able

to produce any macrosopic strain without stretching any beam by applying

Bloch boundary conditions to a unit cell. Here, the same concept is described,

but homogenization theory is used to characterize the periodic truss lattice.

If the periodic truss lattice is assumed to be linear elastic, the elasticity tensor

of the homogenized material is given by the second derivative of the

homog-enized energy density given by Eq. (1.13): _{C} = ∂2_{W}∗_{/∂ε}2_{. Truss lattices}

can be grouped into two categories based on the eigenvalues of the

elastic-ity tensor. If the minimum eigenvalue of the elasticelastic-ity tensor scales with the

stretching stiffness of a beam, this means there are no macroscopic strain

pro-ducing deformations where the beams undergo only bending (otherwise, that

deformation mode would scale like the bending stiffness of a beam, and would

be the minimum eigenvalue). On the other hand, if the homogenized elasticity

tensor has at least one eigenvalue that scales with the bending stiffness of a

beam, then a macroscopic strain-producing deformation mode exists such that

beam, it is called bending-dominated, viz.

min

kεk=1ε·Cε ∼

r

L

2

⇐⇒ stretching-dominated

min

kεk=1

ε·_{C}ε ∼r

L

4

⇐⇒ bending-dominated

(1.14)

in 3D and

min

kεk=1ε·Cε∼

r

L

⇐⇒ stretching-dominated

min

kεk=1ε·Cε∼

r

L

3

⇐⇒ bending-dominated

(1.15)

in 2D. We will use the same nomenclature of bending- and stretching-dominated

lattices to also refer to the individual strain modes, i.e. a strain mode that

has a stiffness proportional to the stretching stiffness of a beam is deemed a

stretching-dominated mode.

Instead of using the ratio r/Lto describe the slenderness of the periodic truss lattice, the relative density, ρ¯, is commonly used, which is the ratio of the volume of solid to air in the periodic truss,

¯

ρ=

P

bVb VUC

, (1.16)

where Vb is the volume of a beam, and VUC is the volume of a unit cell5. The

stiffness scaling relations for bending- and stretching-dominated unit cells are

then commonly expressed as

E∗ ∼Eρ¯b, (1.17)

withE∗ being the smallest elastic modulus of the effective material, andb = 1

for stretching dominated lattices, and b= 3 orb = 2in 2D or 3D respectively.

As a review, for periodic truss lattices,

kinematically determinate ⇐⇒ rigid =⇒ stretching-dominated

bending-dominated =⇒ kinematically indeterminate ⇐⇒ non-rigid.

(1.18)

Figure 1.6 gives examples of rigid, non-rigid, stretching-dominated, and

bending-dominated unit cells of periodic truss lattices.

Stretching-Dominated Bending-Dominated

Bravais Lattice

Multilattice

Figure 1.6: Categorizing lattices and bending- or stretching-dominated lattices and as Bravais lattices or multilattices.

It is important to note here that the term bending-dominated seems to imply

that the deformation of the periodic truss lattice is dominated by the bending

of individual beams, but this is only the case for certain deformation modes.

For instance, the square lattice (see Fig. 1.6) is a bending-dominated lattice

since shear deformations are bending-dominated. However, axial strain in the

x- or y-directions are stretching-dominated modes. Similarly, the hexagon

lattice is a bending-dominated lattice but has a stretching-dominated bulk

modulus, thus the periodic lattice behaves as a nearly incompressible homog-enized material. The entire elastic modulus tensors of select 2D periodic truss

Commonly, periodic truss lattices are also categorized by the number of nodes inside each unit cell of the lattice. In Deshpande et al. [34], lattices with a

single node per unit cell are said to be similarly situated. However here, they are referred to as Bravais lattices, and truss lattices with more than one node per unit cell are called multilattices (see Section 3.1 for more details).

1.5.2 Effective Mechanical Properties

As the stiffness of bending- and stretching-dominated lattices scale differently

with the relative density of the lattice, so do other mechanical properties.

Gibson and Ashby [48] showed that the yield strength of truss lattices also

follows a scaling law with relative density

σ_{y}∗ ∼σyρ¯c. (1.19)

where σ_{y}∗ is the failure stress of the homogenized material, σy is the failure

stress of the constituent material, andc= 1 for stretching-dominated lattices, andc= 2orc= 1.5for bending-dominated lattices in 2D and 3D, respectively. As is the case with the stiffness, the scaling laws apply to specific modes of deformation, rather than the lattice as a whole.

The fracture toughness of truss lattices has also been investigated through

various theoretical and computational techniques. Most of the work on the fracture toughness of truss lattices used expensive structural element

simula-tions [1, 29, 33, 41, 82, 89, 94, 98, 100, 106, 109]. One popular method for

determining the brittle fracture toughness of a lattice is the boundary layer

method [94], which applies the K-field displacements to the boundary of a

large notched lattice (see Fig. 1.7). On the other hand, there has been

ana-lytical work on computing the fracture toughness of lattices. Chen et al. [28]

used effective continuum material models to calculate the corresponding stress

fields around a crack tip, and Lipperman et al. [64] used the representative cell

method of Ryvkin and Nuller [91] to analytically compute the brittle fracture toughness of infinite 2D truss lattices.

All of the work suggests the fracture toughness of a truss lattice has a

power-law scaling with the relative density

K_{IC}∗
σy

√

L ∼ρ¯
d_{,}

(1.20)

Figure 1.7: Depiction of the boundary layer method for a cellular material. Reprinted by permission from Springer Nature: International Journal of Frac-ture [94], copyright 2001.

determined by whether the lattice (or more specifically, deformation mode) is

bending- or stretching-dominated, the fracture toughness scaling law differs

even among lattices in the same class. For instance, the triangle lattice has a

scaling exponent of d= 1, but the kagome lattice has an exponent of d= 1/2, and the hexagon lattice has an exponent of d = 2. For more details on the fracture toughness of truss lattices, see Alonso and Fleck [1].

These scaling laws convey some of the most useful properties of periodic truss

lattices. For instance, a truss lattice made out of a stiff and strong bulk

material (e.g. aluminum), could be used to create an effective material with

a stiffness and strength proportional to the bulk properties and the relative

density of the lattice. If the lattice is made with sufficiently low relative density,

the metamaterial would have the same density as certain foams, but with much

higher stiffness and strength due to the designed microstructure (see Fig. 1.8). These truss lattices open up a new area of the design space for lightweight

materials that are also strong, stiff and tough. Furthermore, periodic truss

lattices can be designed to give certain macroscopic properties (e.g. anisotropy

[104]) simply by changing the topology of the unit cell. This opens up the

possibility of using the same constituent material to manufacture multiple

C h a p t e r 2

### NUMERICAL MODELING OF TRUSS STRUCTURES

2.1 High-Fidelity RVE Characterization

The analysis in Section 1.5 relies on the slender-beam assumption such that

each truss member can be modeled as a linear elastic Euler-Bernoulli beam.

However, non-slender trusses or lattices that undergo large, nonlinear

deforma-tion (e.g. buckling, plasticity, etc.) cannot be analyzed with such simple

models. For this reason, some resort to using more refined microstructural models

-either using nonlinear beams (e.g. [113]) or a full continuum-level finite element

discretization of the unit cell problem in order to better understand the

non-linear constitutive response of the homogenized material [22, 71, 92, 103, 105].

The higher fidelity of continuum-level finite elements allows for the straightfor-ward modeling of higher-order effects (e.g. nodes), material nonlinearity (e.g.

plasticity), and allows for the accurate modeling of other unit cells where beam

theory does not apply (e.g. hollow trusses, general cellular solids).

It is worth noting that if the truss structure is allowed to undergo large

de-formations and/or rotations, then the problem is no longer convex, and the

intractable k-RVE problem Eq. (1.12) must be solved to obtain the nonlinear

response of the homogeneous material. In practice, Eq. (1.12) is

approxi-mated by successively increasing k (i.e. increasing the number of unit cells in the RVE) until the homogenized energy density does not change [113], or by

probing longer wavelength instabilities using Bloch wave boundary conditions

[56].

Meza et al. [71] performed both continuum-level finite element simulations

and simulations using structural elements of various three-dimensional truss

lattices to understand the applicability of beam theory in the linear elastic

regime to different truss lattices. The results showed that the stiffness of non-slender or hollow lattices lattices can differ significantly from beam theory,

but the stiffness of solid slender lattices matched those of beam theory (see

Y

oung'

s Modul

us (MP

a)

100 101 102 103

10-2 10-1

*R*/*L*
2.003

Abaqus Simulations

Timoshenko Beam Simulations Euler-Bernoulli Beam Simulations

Relative Density 101

102 103 104

10-3 10-2 10-1

Figure 2.1: Computed homogenized stiffness of solid (left) and hollow shell (right) octet truss lattices using continuum-level finite element analysis (with the commercial code Abaqus), and structural Euler-Bernoulli and Timoshenko beams for various relative densities. Reprinted from [71].

2.2 Fully-Resolved Simulations

In order to solve boundary value problems of finite-sized truss lattices, some use fully-resolved finite element techniques where the entire truss geometry is

discretized either with continuum or structural finite elements. Of course, the

highest fidelity simulations are those which discretize the truss using

contin-uum finite elements (e.g. [104], or shell elements in the case of hollow lattices

[73]; see Fig. 2.2), and can be used to model geometric and material

nonlinear-ity. However, the computational cost of these simulations limits the size of the

truss that can be modeled. Recently, there has also been an effort to creating

reduced-order models of nodes of non-slender truss lattices in order to capture

the higher-order effects while keeping computational costs low, enabling the modeling of larger lattices [81].

Simulations that use structural finite elements (e.g. with each truss member

modeled with a beam finite element) are less expensive and can be used to

model larger truss lattices [1, 29, 33, 41, 53, 78, 82, 89, 94, 100, 106, 107].

Fully-resolved structural finite element models have the ability to incorporate

geometric and material nonlinearities, as well as the ability to model more

general non-periodic truss lattices. However, the number of structural elements

that can be modeled is still limited due to the computational cost. As the sheer number of truss members contained in such truss lattices disqualifies

brute-force modeling techniques due to extreme computational expenses, multiscale

Figure 2.2: Simulation of uniaxial tension of a notched hollow octet truss lattice modeled using shell finite elements to investigate the insensitivity of truss lattices to flaws. Reprinted from [73].

2.3 Numerical Homogenization

One of the most common techniques for solving multiscale boundary value

problems like Eq. (1.9) is that of numerical homogenization. It attempts to

approximate solutions to the homogeneous problem in Eq. (1.10). Since finding

a closed-form solution to Eq. (1.11) (or Eq. (1.12) if the energy is nonconvex)

is generally not possible, the microscale RVE problem is solved numerically

in order to compute W∗(∇u) or its derivatives — coupling the two scales. Figure 2.3 gives an example of the numerical homogenization approach and

shows the coupling between scales. Since the macroscale and microscale are

treated separately, there is an inherent assumption of a separation of scales

between the micro- and macro-scale (i.e. 1). Therefore, these techniques are referred to as a hierarchical multiscale techniques.

One of the most well-known numerical homogenization techniques is the FE2 method [39, 47]. In the FE2 method, the finite element method is used to approximate both the homogenized problem, Eq. (1.10), and the RVE problem,

Eq. (1.11) (or Eq. (1.12) is approximated if the energy density is not convex).

For trusses, the macroscale BVP is usually approximated with continuum finite

elements, while structural finite elements are used to model the truss in the

RVE [7, 76, 79, 113]. There are also some models that use a higher-order

version of the RVE problem that depends on the deformation gradient, F,

and its gradient, thereby introducing a length scale into the problem [35, 38,

Figure 2.3: Pictorial description of numerical homogenization reprinted from Matouš et al. [67] with permission of the copyright holder, Elsevier. FM

rep-resents the macroscopic deformation gradient, andSM andCM represent the

macroscopic stress and tangent matrices that are returned to the macroscale after solving the RVE problem.

Another way of thinking about these hierarchical multiscale methods is that

they aim to approximate the solution of the heterogenous fine-scale problem by

looking for solutions through asymptotic expansion. For the case of first-order

homogenization (i.e. where strain gradients are not included), the methods

look for a solution of the form [30]

u(x) = u(x) +v

x,x

+O(2), (2.1)

where u is the smooth displacement computed from the homogenized

bound-ary value problem, and v represents the fine-scale periodic oscillations

com-puted from the RVE problem.

One contention with these hierarchical multiscale methods like FE2 _{is that}

the essential boundary conditions are only satisfied in an average sense. It is

desired to enforce u(X) = u0(X) on the boundary, but FE2 only enforces

u(X) = u0(X). Since the average of v over a unit cell is zero, the displace-ment field averaged over a unit cell at the boundary satisfies the essential boundary conditions rather than the fine-scale displacement field itself. In

lin-ear elasticity, however, the energy difference between the two-scale expansion

that FE2 matches the global behavior of the body, but it does not capture boundary effects.

Similar to how the FE2 _{method does not satisfy boundary conditions exactly,}

it also does not exactly enforce compatibility of the displacement field. For

instance, take two elements K1 and K2 in the macro-scale finite element

dis-cretization. At the edge ∂K12 between the two elements, in the two-scale

ex-pansion Eq. (2.1), we have uK1_{(}_{x}_{) =}_{u}K2_{(}_{x}_{)}_{(due to conformity of the shape}
functions on the macro-scale) but vK1_{(}_{x}_{)} _{6=} _{v}K2_{(}_{x}_{)}_{, since} _{v}_{(}_{x}_{)} _{depends on}

∂u

∂x which is not necessarily the same in K1 and K2. The displacement field

is only conforming on the macro-scale, but not on the microscale. The

dis-placement field is conforming at element boundaries in the same way that it

satisfies boundary conditions: the displacement field averaged over a unit cell

is conforming. One could make similar arguments to those made above with

the boundary conditions that this lack of conformity does not incur large errors

in the solution as long as the separation of scales holds.

2.4 Quasicontinuum Method

Another multiscale modeling technique that is gaining interest in the truss

lat-tice modeling community is the Quasicontinuum (QC) method — aconcurrent

multiscale technique that does not require a separation of scales. Although

originally developed to efficiently model atomic crystals [101], the QC method has recently been applied to truss lattices [15–20, 86–88]. Unlike numerical

homogenization methods, the QC method starts from a finite-sized lattice,

then applies kinematic constraints and energy approximation techniques (also

calledsummation rules orsampling rules) to drastically reduce the number of degrees of freedom (dofs) and the computational costs associated with

eval-uating the mechanical quantities. In regions of interest (e.g. large strains,

plasticity, etc.), the kinematics and the energy of the lattice are computed

exactly, while in regions of less interest, the kinematic constraints and energy

approximation techniques are used to approximate the behavior of the lattice.

The kinematic constraints in the QC method are developed by choosing repre-sentative sites (commonly called repatoms in atomstic simulations and repn-odes for trusses) which retain all of their dofs, and dofs of the remaining lattice

sites are interpolated from the representative sites (see Fig. 2.4). Most

Figure 2.4: The traditional QC method for atomic lattices (left) and the ex-tension to truss lattices (right).

there have been formulations with more complex interpolation schemes such

as meshless methods [111] and higher-order interpolations [16, 114]. While

there are relatively few unique interpolation schemes, there are a wide variety

of QC techniques used to approximate the global energy of the lattice.

The first distinction of the QC methods comes from the so-called local and

nonlocal treatment of coarse-grained regions in the simulation. Local regions of the simulation are regions where the energy of the lattice is approximated

using only the deformation gradient at a given point. Usually, this is done

using the Cauchy-Born rule — an assumption that the neighboring lattice

sites undergo affine deformation (in addition to relative shifts of the lattices in

the multilattice) defined by the deformation gradient at a point. In nonlocal

regions of the simulation, no such assumption is made, and the energy of the

lattice is computed exactly by using the true kinematics of the lattice.

rule is used to approximate the energy. There are also fully local versions of the QC method where the Cauchy-Born rule is used everywhere [99].

How-ever, these methods are extremely similar to the numerical homogenization

methods with a single atom as the unit cell, and molecular statics (MS) is

used to compute the energy of the unit cell problem (so a suitable name would

be FE-MS). Lastly, there arefully-nonlocal versions of the QC method, where no distinction is made between the fully-resolved regions and coarse-grained

regions [2, 3, 37].

Various methods have been proposed for sampling the mechanical quanti-ties (such as energy and forces) in the coarse-grained regions including local,

Cauchy-Born-type approximations [101], force- and energy-based summation

rules [37], cluster sampling [58], numerical quadrature [49], and combinations

of Cauchy-Born and nonlocal sampling rules [3]. It should be noted that all of

these summation rules are ad-hoc, developed for a specific interpolation rule

— usually linear interpolation on a Delaunay triangulated mesh — and do not

naturally generalize to higher-order interpolations.

Most implementations of the QC method are intended to work specifically

with Bravais lattices. That is, lattices where all atoms or nodes of a truss lie

on sites in the lattice set

ΛB =

(

X ∈_{R}d
X =

d

X

j=1

bjaj+S, bj ∈Z

)

, (2.2)

whereaj are the primitive lattice vectors, and S represents a rigid body shift

of the entire lattice. However, there are a few instances of the QC method

used for more complex atomic lattices 1 [102], which have atoms that lie on the sites in the set

ΛM =

(

X ∈_{R}d
X =

d

X

j=1

bjaj +Sα, bj ∈Z, 1≤α≤nB

)

. (2.3)

This set can be described as being made up of nB Bravais lattices shifted

relative to one another by the shift vectors Sα. Therefore, it is common to

refer to these lattices asmultilattices. Hexagonal close packed (HCP) crystals are an example of an atomic multilattice, and the hexagon and kagome trusses

are examples of 2D truss multilattices (see Fig. 3.1).

The first implementation of the QC method for multilattices in Tadmor et al. [102] is a local-nonlocal version of the QC method. In the fully-resolved region,

each unit cell location was given extra dofs δα, α ∈ {1, . . . , nB} representing

the relative shifts of thenB additional atoms at each unit cell site (the shift of

the first Bravais lattice was defined to be zero,δ1 =0). However, in the coarse-grained region, sites only contained d dofs in d dimensions, and the atomistic

equivalent of the RVE problem, Eq. (1.11), with a single unit cell was solved in

each coarse-grained element. Since the atomic interactions are non-convex, the

method was improved to approximate the atomistic equivalent of the k-RVE

problem, Eq. (1.12), using a method called cascading Cauchy-Born kinematics [36]. Cascading Cauchy-Born kinematics uses Bloch wave techniques to probe

instabilities with wavelengths longer than a single unit cell, and allows more

unit cells to be incorporated into the RVE. This allows the local-nonlocal QC

method to capture phase transformations in the coarse-grained regions.

The extension of the traditional atomistic QC method to model truss lattices

is rather straightforward: nodes of the truss replace atoms, and finite

ele-ment beam or bar energies are used in place of inter-atomic potentials (see

Fig. 2.4). Initial studies assumed the truss members to behave as linear elas-tic springs; later extensions included inelaselas-ticity and failure of truss members

[18, 19, 59, 86] as well as introducing rotational dofs at each node and

us-ing Euler-Bernoulli beam connections to model the stretchus-ing and bendus-ing of

truss members [16]. Concepts were further paired with the eXtended Finite

Element Method (XFEM) to track the propagation of cracks in the lattice

(see Fig. 2.5) [88]. However, all of these implementations have been limited to

local-nonlocal versions of the QC method only for trusses that can be defined

by a 2D Bravais lattice (either square or cross-braced lattices).

2.5 Shortcoming of Existing Methods

While there has been an extensive amount of work devoted to numerical

mod-eling of truss structures, there is still a gap in the modmod-eling capabilities.

Fully-resolved continuum finite element models are the highest fidelity models

— capable of capturing strong material nonlinearity and not requiring any

assumption on the slenderness of truss members — but are extremely expensive

to solve, limiting the size of the simulation [73, 104]. Fully-resolved structural

Figure 2.5: The QC method paired with aspects of the extended finite element method to model the crack propagation (crack path shown in red) in a cross-braced truss lattice. Reprinted from Rokoš et al. [88] with permission from the copyright holder, Elsevier

to reduce the number of degrees of freedom needed to model finite-sized truss

lattices. By using sophisticated beam elements, it is even possible to model

geometric as well as material nonlinearity, and non-periodic truss lattices.

However, even though structural finite elements are inexpensive compared to continuum-level finite element descriptions, modeling multiscale metamaterials

using structural elements is not a scalable approach.

Modeling representative volume elements using either high-fidelity continuum

finite elements or less expensive structural finite elements is useful in

charac-terizing the properties of the effective material. However, whether the RVE

computations are done "offline" to characterize the homogenized energy

den-sity or "online" in the FE2 method to solve boundary value problems, there are problems with strong nonlinearities (stemming from the intractability of the k-RVE problem Eq. (1.12)). Furthermore, the homogenization procedure

com-pletely fails when there are shear-band instabilities at the microscale because

there is no length scale to regularize the solution. Homogenization strategies

such as FE2_{also have the additional issue of not satisfying boundary conditions}

exactly and therefore do not accurately capture boundary effects.

The QC method lies in a middle ground between fully-resolved models and

hierarchical multiscale models. Since it starts with the fully-resolved model,

the QC method is able to capture significant nonlinearities (buckling, shear bands, failure of individual trusses, etc.) and boundary effects in certain

fully-resolved regions, while the coarse-graining techniques enable the method to

scale up to truly multiscale lattices. The initial work in using the QC method

to model trusses is promising, but so far it has only been used to model

kinematics.

The remainder of this thesis is dedicated to filling the gaps in existing modeling

methods by developing a formulation of the QC method to accurately model

the nonlinear response of general trussmultilattices inthree dimensions. The novelfully-nonlocal multilattice formulation allows for general truss models to be used, and will be paired withgeometrically nonlinear beam descriptions to model buckling of the truss without any separation of scales assumptions or

solving microscale RVE problems. The method will be implemented with an

C h a p t e r 3

### FUNDEMANTALS OF THE QUASICONTINUUM METHOD

A significant portion of this chapter is taken from our recent publication:

Gregory P. Phlipot and Dennis M. Kochmann. A quasicontinuum theory forthe nonlinear mechanical response of general periodic truss lattices.Journal of the Mechanics and Physics of Solids, 124:758 – 780, 2019. ISSN 0022-5096. doi: https://doi.org/10.1016/j.jmps.2018.11.014. URLhttp://www.sciencedirect. com/science/article/pii/S0022509618304071.

3.1 Initial Problem Statement

In this section, we outline the fully-resolved problem that will later be approx-imated with the QC method. The purpose of this section is to give definitions

of unit cells, truss elements, nodes, and the total potential energy of the system

which will be used in the rest of the thesis.

Periodic truss lattices, i.e. cellular networks composed of beams and beam

junctions (referred to as nodes in the following), are produced by periodically
repeating a unit cell along directions A = {a1, . . . ,ad} with basis vectors
a ∈ _{R}d _{in} _{d} _{dimensions. A lattice} _{Ω} _{is defined through the set of nodes,} _{P}_{,}

and the set of truss members1, E, i.e. Ω ={P,E}. For convenience, the body of interest is decomposed into a set of unit cells. A unit cell at a location Xu

(in the undeformed configuration) can be defined by the set of points,Pu, that

lie inside the volume spanned by vectorsAand centered at Xu (see Fig. 3.1a),

i.e.

Pu =

(

X ∈ P | X =

d

X

i=1

Xu+tiai, ti ∈

−1 2,

1 2

for i= 1, . . . , d

)

.

(3.1)

The unit cell also contains the set of truss members that connect the points in Pu to each other, Eu, and the set of truss members interacting with points

in neighboring unit cells, En

u.

For some truss lattices, (e.g. square, triangle) each unit cell consists of only

a single node with connections only to nodes in neighboring unit cells (i.e.